# – Polymerization Kinetics ```Polymerization Kinetics –
Can: (a) derive rate expressions (monomer usage, e.g.); (b) derive MWD;
(c) predict concentrations as functions of time (batch) or residence time (,
continuous flow).
Rate, mechanism, elementary step:
Consider simple initiation of a poly. –
I  2 R
R + M  M
(rate constant = k1)
(k2)
r1 = k1 [I]
r2 = k2 [R] [M]
Elementary = mechanistic = rates of reaction given by stoich.
But tells us nothing about how the concs. change. – need an “overall rate”
for this.
Overall rate:
Consider R -- 2 mols formed in r1, 1 mol used up in r2
So r R = 2 r1 – r2
Kinetics, k1 ~ k2
Conc., kmol/m
3
0.01
0.008
0.006
[I]
[R&middot;]
0.004
0.002
0
0
50
100
150
200
time, s
Kinetics, k1 &lt;&lt; k2
Conc., kmol/m
3
0.01
0.008
0.006
[I]
[R&middot;]
0.004
0.002
0
0
50
100
150
200
time, s
Case 2 more common – intermediate forms slow, decomposes fast.
After short setup time, d[R]/dt ~ 0
, for long time
So SSA: For all unstable intermediates R , at t = 0+ , d[R]/dt ~ 0 and:
r R = 0
- hard to find any radicals
- see some polymer immediately
So all intermediates must be in “steady state”, even if the overall process is
NOT.
Typical mechanism:
I  2 R
(rate constant = k1)
R + M  M1
(k2)
M1 + M  M2
(kp1) p for propagation
M2 + M  M3
(kp2) etc.
Eventually:
Mj + Mk  Pk+j
or
Pk + Pj (kt, termination)
X + Mj  X + Pj
(ktr, chain transfer)
X + M  M1
(kx, chain transfer)
Can also have chain transfer to monomer itself, or to polymer (common,
leads to branching), or to initiator. Chain transfer is a more reliable method
of MW control in many addition polys.
Kinetics analysis of above –
- R , M1 , Mj , X all unstable
r R = 2 r1 – r2 ~ 0
rtr = ktr [X]  [Mj]
rX = rtr - rX ~ 0
rM1 = +r2 – rP1 - ktr [X] [M1] + rX - kt [M1] [Mj] ~ 0
rM2 = -rP2 + rP1 - ktr [X] [M2]
- kt [M2] [Mj] ~ 0
etc.
rP = ktr [X] [Mj] + kt [M1] [Mj] + kt [M2] [Mj] + kt [M3] [Mj]
+…
rP = ktr [X] [Mj] + kt ( [Mk]) ([Mj])
Now add the “zero” terms rX , rM1 , rM2 etc.
0 ~ +r2 – rP - kt ( [Mk]) ([Mj])
We reject
rP on physical grounds, and recognize that a “j” and “k”
polymer describe the same thing, and so write (using r R eqn.):
[Mj] = (r2/kt)0.5 = (2r1/kt)0.5 = [M]
Since r1 is usually slow (often so slow that [I] ~ constant), this represents a
measurable quantity, an “observable”.
Now can subs. [M] into rp to get the total poly. rate, in terms of
observables. The total rate at which monomer is used up is approx. the
sum of the propagation terms (long chain approximation), because almost
all monomer used up in propagation. If we then assume:
kp1 ~ kp2 ~ kp3 etc. – just kp
-rM = kp [M] [Mj] = kp (2r1/kt)0.5 [M]
Relationship between kinetics, MWD:
XN

# mols monomers used

# mols polymer
(instantaneous)
Using the above e.g. –
XN

 rM

rP
1 (2 r1 k t ) 0.5

X
k p [M ]
k P [M ]
k tr [ X ]  k t [M ]

k tr [ X ]
k p [M ]
 ( propagation rates)
 (ter min ation rates)
E.G. 1 – Finding a polymer distribution, heuristic method – Radical, term.
by combination
Key relationship 
j 1
 [M
j 1 k 1
j k
] [ M k ] 

 [M
j 2
j 1
]2 

 [M
j 1
j
]2
Other keys –
(a) Pj mol fraction at time t = (rate to Pj)/( rates to all Pk)
(b) Schulz-Flory assumed for the living chains
Kinetics of Step Poly. - good e.g., detailed mechanisms - http://www.pslc.ws/mactest/level4.htm
for poly(carbonate) or poly(urethane).
Note that a small molecule need not condense out; if not, either limits MW
or requires solvent (why?).
Kinetics and MWD:
http://www.engin.umich.edu/~cre/07chap/html/polymerization.pdf simplest e.g., stoich. balance
Note that “p” here doesn’t represent a constant prob. wrt time; it is constant
wrt all chains.
Therefore question is: do all chains see same “environment” at any time t?
[yes, batch reactor; no, continuous stirred tank reactor]
The form of: XN suggests Schulz-Flory (doesn’t prove it), but it’s
proven below. The math is far more complex for case of stoich. imbalance
of reactive groups, but this is not common.
Stoich. imbalance – see
http://www.engin.umich.edu/~cre/07chap/frames.htm , section I.E
Kinetics of a catalyzed step poly. – see
http://www.engin.umich.edu/~cre/07chap/frames.htm , section I.E
Polymerization Reactor Design
For most polymerizations, the key considerations are:
 Type reactor – batch or continuous (CSTR) ; bulk, solution,
suspension, emulsion?
 Temperature – useful range usually narrow
 Initiator, catalyst, chain transfer agent (“modifier”, “endblocker”)
concentrations.
 Phase equilibria during the reaction – will polymer precipitate?
 Purity of feed
 Agitation – especially at high viscosity
All have an effect not only on the average MW’s, but also on MWDs.
The basic mass balances:
F j  F jo   j
dN j
dt
 j
r1 V
r V
(CSTR)
(batch)
where:
Fj = molar flow rate of component j = Cj F' = concentration * volumetric flow
rate
Nj = number mols of component j
j = stoichiometric number of j (e.g., plus for product, minus for reactant)
V = volume of the active phase (NOT the reactor)
Subscript “o” = feed; “1” = exit stream
r = the reaction rate expression
The equations give very different results for most types of polymerizations.
For the CSTR and PFR, the quantity that is analogous to time is the “space
time”, V/v0 = 
General Rule for MWDs of Polymerizations –
Let  = the average time a chain is growing (including crosslinks). If:
(a)  &gt;&gt; t (batch) or  (CSTR), then a change in t or  has a great effect
on MWD, and so a batch reactor will produce the narrower MWD,
because all chains see the same growth time.
(b)  &lt;&lt; t (batch) or  (CSTR), then a change in t or  has less effect on
MWD, and a CSTR will produce the narrower MWD, because all
chains see the same local composition.
Examples –
(a) Step (condensation) polymerization (is long). Typical MWD (Wj =
weight of polymer with j units) for a batch (solid line) and a CSTR
(dashed line) are shown. The batch typically gives the Flory (most
probable) distribution with polydispersity near 2 (p = monomer
conversion).
Wj
j
Now the CSTR gives the narrower MWD, which is often near a Flory
(most probable) distribution – see graph below.
“Living”
(c)
Polymerizations
–
anionic,
cationic
or
metallocene
polymerizations with little of no termination –  can be long
Addition copolymerizations – not so easy – “local composition”
(d)
considerations may apply, because may want copolymer at specific A/B
ratio.
Mathematics of the Flory Distribution, addition poly.
For no combination:
p
propagation rate
 (ter min ation and propagation rates)
XN

 (term.  propag. rates) ~ ( propag.)
(term.)
 term. rates
1

1  p
Can also be derived statistically:
yj = mole fraction j-mer = (1-p) pj-1
Note: w j 
X w   j wj 
yj M j
y
j
Mj

j p j 1
 j p j 1
 (1  p) 2 j p j 1
1 p
1 p
The batch reactor can be modeled as an average of several Flory
distributions
t
Cp


0
1 (d [ M ])
dt
XN
t
dt 
  (ter min ation
rates) dt
0
If we consider that the propagation rate &gt;&gt; initiation rate for most
polymerizations (“long chain approximation”), it is easy to get this equation
from the one preceding it.
(e) Addition polymerization with chain branching.
This is a harder case. For many addition polymerizations, is short. But
chain branching reactions usually take place over a long time. The following
data were collected for vinyl acetate polymerization with chain branching:
The y-axis is:
X w / X N . The X-axis is fraction conversion.
Clearly the batch reactor is superior, which means that the slower branching
reaction controls the MWD ( is long).
Fortunately, many CSTRs don’t
behave as perfectly mixed in real polymerizations.
They exhibit
“segregation”, a state of imperfect mixing, especially when the viscosity gets
high. We see here that the imperfect mixing actually produces a narrower
MWD.
When is a Batch Reactor not a Batch Reactor?
Consider the following case.
We have an addition polymerization in
suspension, constant T.  is short. But all of the polymer precipitates as
soon as it’s formed. What happens to the concentration of monomer, CM?
CM = NM / V
While NM is certainly decreasing, V (the “active” phase, not the entire
suspension) also decreases proportionally, because it’s almost all monomer.
Therefore, assuming excess initiator, the rate remains constant also. This
means the batch reactor behaves exactly like the CSTR for this case.
Real suspension polymerizations seldom behave exactly like this, because
there is usually some polymer solubility in the monomer (and vice-versa).
But there is often little enough that CM changes little. This means the batch
reactor can give narrow MWD for suspension polymerization (and its cousin,
emulsion polymerization), even when  is short.
Complications in Polymerizations at High Conversion
E.g., addition polymerizations often have observed kinetics that differ from
1st order in monomer.
r 
[M]2
Ln(1-X)
r 
[M]0
time
Above e.g. for Addition Poly. –
[M]0-0.5 - Trommsdorff effect – restricted termination – kt  [M]1-2
[M]2 – Glass effect – restricted propagation - kp  [M]
Both actually mass transfer effects, but often modeled “kinetically”.
```